organic inorganic composites of semiconductor of the excitons. these excitonic processes are...
Post on 26-May-2020
Embed Size (px)
Organic−Inorganic Composites of Semiconductor Nanocrystals for Efficient Excitonics Burak Guzelturk and Hilmi Volkan Demir*
Department of Electrical and Electronics Engineering, Department of Physics, UNAM − Institute of Materials Science and Nanotechnology, Bilkent University, Ankara 06800, Turkey
LUMINOUS! Center of Excellence for Semiconductor Lighting and Displays, TPI − The Photonics Institute, School of Electrical and Electronic Engineering, School of Physical and Materials Sciences, Nanyang Technological University, Singapore 639798, Singapore
ABSTRACT: Nanocomposites of colloidal semiconductor nanocrystals integrated into conjugated polymers are the key to soft-material hybrid optoelectronics, combining advantages of both plastics and particles. Synergic combination of the favorable properties in the hybrids of colloidal nanocrystals and conjugated polymers offers enhanced performance and new functionalities in light-generation and light-harvesting applications, where controlling and mastering the excitonic interactions at the nanoscale are essential. In this Perspective, we highlight and critically consider the excitonic interactions in the organic−inorganic nanocomposites to achieve highly efficient exciton transfer through rational design of the nanocomposites. The use of strong excitonic interactions in optoelectronic devices can trigger efficiency breakthroughs in hybrid optoelectronics.
Both colloidal semiconductor nanocrystals (NCs) and π-conjugated semiconductor polymers (CPs) are attractive materials for a broad range of applications including bioimaging,1,2 sensing,3,4 electronics,5,6 and photonics.7,8
Using these emerging materials for energy-efficient lighting, display and photovoltaic technologies have gained escalating interest in the past 2 decades.9−12 To this end, combining favorable optical properties of the colloidal semiconductor NCs and versatile physical properties of the conjugated polymers in hybrid platforms offers enabling opportunities for high- performance devices along with new functionalities. For this purpose, in the organic−inorganic composite systems, control- ling the photophysical properties becomes crucial. These properties principally comprise excitons and excitonic pro- cesses, which include exciton formation, diffusion, transfer, and dissociation as well as radiative and nonradiative recombination of the excitons. These excitonic processes are schematically depicted in Figure 1. An exciton, which is a Coulombically bound electron−hole
pair, is the primary form of the excited-state energy in the CPs and the NCs. An exciton can be created via either optical or electrical excitation (Figure 1a). Optical excitation occurs through absorption of a photon, while electrical excitation requires simultaneous injection of an electron and a hole. Within the lifetime of an exciton, it may radiatively or nonradiatively recombine (Figure 1b). Radiative recombination results in emission of a photon, whereas nonradiative recombination does not produce light but heat. Exciton diffusion (Figure 1c) is another process that is widely observed in the close-packed solid films of the CPs and the colloidal NCs. In the case of CPs, exciton diffusion/migration can
happen either via exciton hopping within the delocalized excited-state landscape of CP13 or via Förster resonance energy transfer (FRET) between different chromophoric units of the CP.14,15 In the colloidal NCs, exciton diffusion dominantly takes place through long-range nonradiative energy transfer because excitons are confined to the NCs.16,17 The exciton diffusion length in the CPs and the NCs is typically on the order of 10 nm.10,17 For a solar cell, attaining a longer exciton diffusion length is desired for enhanced light-harvesting performance.18,19 In the case of a light-emitting diode (LED), exciton diffusion is undesired because it can cause trapping of the excitons at the trap/defect sites (Figure 1c), causing nonradiative recombination.
At the interfaces of materials having energetically staggered band alignment, excitons might dissociate through charge transfer. This process involves spatial overlap of the wave functions between different materials that are in close proximity (
reactive species through formation of free charge carriers, which finds use in photovoltaics for charge separation. On the other hand, in electroluminescent devices, it is essential to control the recombination zone of the excitons within which they radiatively recombine. The management of the exciton recombination zone can be achieved through excitation energy transfer (Figure 1e) including FRET,20 which is a near-field dipole−dipole coupling between the species that are in close proximity (typically
donors for the QDs. This nonradiative energy transfer from the CP into the QD was also verified by photoluminescence excitation (PLE) spectroscopy.41 PLE of the QD emission was shown to exhibit strong enhancement in the spectral range, where the CP has strong absorption, owing to the exciton transfer from the CPs into the QDs. Other evidence of this type of exciton transfer was shown by the slower rise time of the fluorescence decay in the acceptor QDs due to exciton feeding from the CPs.46 Different from the early works, which generally focused on blended CP−QD films, Lutich et al. have investigated nonradiative energy transfer in an electrostatically integrated CP−QD hybrid.48 They have demonstrated that FRET is the dominant excitonic mechanism among others (Dexter energy transfer and charge transfer), with an efficiency as high as 80% despite a type-II band alignment between the CP and the QD.48
Later, Stöferle et al. put forward that exciton diffusion is crucially needed for nonradiative energy transfer to take place from the CPs into the QDs.51 With the help of exciton diffusion in the organic part, excitons would become effectively closer to the acceptor QDs (see Figure 2a) so that nonradiative energy transfer would be more efficient.65,66 In this aforementioned work, exciton-diffusion-assisted exciton transfer was demon- strated in blended CP−QD films by measuring the transfer efficiencies as a function of temperature. At low temperatures, exciton-transfer efficiency was found to be suppressed (see Figure 2b) due to temperature deactivation of the exciton diffusion in the CPs. Thus, at low temperatures, exciton
diffusion could not assist exciton transfer. However, ref 51 considered only blended CP−QD films having QD density as low as 3 wt %. This low density was intentionally set to prevent possible phase segregation, which is a common phenomenon in the blended CP−QD films.26,40,62,63 At increased QD densities in a polymer matrix, the QDs will
form micron-scale aggregates in this polymer matrix. The phase segregation is detrimental against efficient nonradiative energy transfer because the donor CPs and the acceptor QDs are physically separated. Eventually, crucially exciton-diffusion- assisted exciton transfer in the CP−QD composites was restricted with the observation only in blends incorporating low QD density, where exciton transfer is not strong. The interplay between exciton diffusion and exciton transfer had not been understood in the hybrid CP−QD nanocomposites. To this end, we have developed hybrid CP−QD nanocomposites using functionalized CPs that have anchor groups facilitating strong attraction to the QD surfaces; thus, these hybrids substantially suppress phase segregation even for the QD densities up to 80 wt %.40
Previously, different hybridization methods have been used to integrate the QDs and the CPs together, including ligand exchange of QDs with CPs or synthesizing QDs in a CP-based ligand medium.55,67,68 These methods generally do not preserve high-quality optical properties of the QDs and may cause exciton dissociation and charge transfer due to intimate contact between the organic and inorganic species.45 Therefore, using core/shell QDs together with functionalized CPs having anchor
Figure 2. (a) Schematic demonstration of exciton-diffusion-assisted nonradiative energy transfer from a conjugated polymer into a colloidal QD. An exciton generated in the disordered density of states of a conjugated polymer can diffuse via hopping with the help of activation energy (kT). Exciton diffusion assists nonradiative energy transfer to a QD from the conjugated polymer. (b) Temperature-dependent nonradiative energy-transfer efficiencies in the blended CP−QD films having a QD density of 3 wt %. Adapted with permission from ref 51. Copyright 2009, American Chemical Society.
Figure 3. Nonradiative energy-transfer efficiencies as a function of temperature for (a) functionalized CP−QD hybrid and (b) nonfunctionalized CP−QD blended films at low (3 wt %) and high (45 wt %) QD densities within in the polymer matrix. Reproduced from ref 40 with permission from The Royal Society of Chemistry.
The Journal of Physical Chemistry Letters Perspective
DOI: 10.1021/acs.jpclett.5b00415 J. Phys. Chem. Lett. 2015, 6, 2206−2215
groups stands out as an attractive route to boost exciton transfer in the hybrids while preserving the favorable optical properties of the QDs. To date, generally amine,60 carboxyl,40
and thiol62,63 groups (see Table 1) have been used in the functionalized CPs as the anchor groups. This type of hybridization will be promising for future hybrid organic− inorganic optoelectronic systems. In our previous work employing hybrids of the functionalized
CPs and the QDs, we achieved phase-segregation free hybrids having QD densities up to 80 wt %.40 By this means, nonradiative energy transfer from the CPs into the